Créer une présentation
Télécharger la présentation

Télécharger la présentation
## Chapter 3: Structures via Diffraction

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -

**Chapter 3: Structures via Diffraction**• Goals • – Define basic ideas of diffraction (using x-ray, electrons, or neutrons, which, although they are particles, they can behave as waves) and show how to determine: • Crystal Structure • Miller Index Planes and Determine the Structure • Identify cell symmetry.**Chapter 3: Diffraction**Learning Objective Know and utilize the results of diffraction pattern to get: – lattice constant. – allow computation of densities for close-packed structures. – Identify Symmetry of Cells. – Specify directions and planes for crystals and be able to relate to characterization experiments.**CRYSTALS AS BUILDING BLOCKS**• Some engineering applications require single crystals: --turbine blades --diamond single crystals for abrasives Fig. 8.30(c), Callister 6e. (Fig. 8.30(c) courtesy of Pratt and Whitney). (Courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission.) • Crystal properties reveal features of atomic structure. --Ex: Certain crystal planes in quartz fracture more easily than others. (Courtesy P.M. Anderson)**POLYCRYSTALS**• Most engineering materials are polycrystals. Adapted from Fig. K, color inset pages of Callister 6e. (Fig. K is courtesy of Paul E. Danielson, Teledyne Wah Chang Albany) 1 mm • Nb-Hf-W plate with an electron beam weld. • • Each "grain" is a single crystal. • • If crystals are randomly oriented, • overall component properties are not directional. • • Crystal sizes range from 1 nm to 2 cm • (i.e., from a few to millions of atomic layers).**Diffraction by Planes of Atoms**Light gets scattered off atoms…But since d (atomic spacing) is on the order of angstroms, you need x-ray diffraction (wavelength ~ d). To have constructive interference .**(c) 2003 Brooks/Cole Publishing / Thomson Learning**Figure (a) Destructive and (b) reinforcing interactions between x-rays and the crystalline material. Reinforcement occurs at angles that satisfy Bragg’s law.**Diffraction Experiment and Signal**Scan versus 2x Angle: Polycrystalline Cu Diffraction Experiment Measure 2θ Diffraction collects data in “reciprocal space” . How can 2θ scans help us determine crystal structure type and distances between Miller Indexed planes (I.e. structural parameters)?**(c) 2003 Brooks/Cole Publishing / Thomson Learning**Figure: (a) Diagram of a diffractometer, showing powder sample, incident and diffracted beams. (b) The diffraction pattern obtained from a sample of gold powder.**Figure : Photograph of a XRD diffractometer. (Courtesy of**H&M Analytical Services.)**Crystal Structure and Planar Distances**h, k, l are the Miller Indices of the planes of atoms that scatter! So they determine the important planes of atoms, or symmetry. Distances between Miller Indexed planes For cubic crystals: For hexagonal crystals:**Allowed (hkl) in FCC and BCC for principal scattering (n=1)**Self-Assessment: From what crystal structure is this? h + k + l was even and gave the labels on graph above, so crystal is BCC.**Example from Graphite**Diffraction from Single Crystal Grain Mutlple Grains: Polycrystal Powder diffraction figures taken from Th. Proffe and R.B. Neder (2001) http://www.uni-wuerzburg.de/mineralogie/crystal/teaching/pow_a.html**Example from Aluminum**Diffraction from Mutlple Grains of Polycrystalline Aluminum Powder diffraction figures taken from Th. Proffe and R.B. Neder (2001) http://www.uni-wuerzburg.de/mineralogie/crystal/teaching/pow_a.html**Example from QuasiCrystals**Remember there is no 5-fold symmetry alone that can fill all 3-D Space!**SUMMARY**• Materials come in Crystalline and Non-crystalline Solids, as well as Liquids/Amoprhous. Polycrystals are important. • Crystal Structure can be defined by space lattice and basis atoms (lattice decorations or motifs), which can be found by diffraction. • Only 14 Bravais Lattices are possible (e.g. FCC, HCP, and BCC). • Crystal types themselves can be described by their atomic positions, planes and their atomic packing (linear, planar, and volumetric). • We now know how to determine structure mathematically and experimentally by diffraction.**Example: Examining X-ray Diffraction**The results of a x-ray diffraction experiment using x-rays with λ = 0.7107 Å (a radiation obtained from molybdenum (Mo) target) show that diffracted peaks occur at the following 2θ angles: Determine the crystal structure, the indices of the plane producing each peak, and the lattice parameter of the material.**Example 3.20 SOLUTION**We can first determine the sin2 θ value for each peak, then divide through by the lowest denominator, 0.0308.**Example 3.20 SOLUTION (Continued)**We could then use 2θ values for any of the peaks to calculate the interplanar spacing and thus the lattice parameter. Picking peak 8: 2θ = 59.42 or θ = 29.71 Å Å This is the lattice parameter for body-centered cubic iron.